and low-cost AlNi catalysts for hydrogen production Use of ... 2156665:3/... Use of ultrasonic...
Embed Size (px)
Transcript of and low-cost AlNi catalysts for hydrogen production Use of ... 2156665:3/... Use of ultrasonic...
Use of ultrasonic cavitation for near surface structuring of robust and low-cost AlNi catalysts for hydrogen production
P. V. Cherepanova, I. Melnyka, E. V. Skorbb, P. Fratzlb, E. Zolotoyabkoc, N. Dubrovinskaiad, L. Dubrovinskye, Y. S. Avadhutf, J. Senkerf, L. Leppertg, S. Kmmelg, and D. V. Andreevaa
I. Aluminum-Nickel binary phase diagram
Fig. S1 shows the aluminum-nickel binary phase diagram (Al-Ni BPD). The used
composition is 50:50 wt. % (shown by the gray line).
Fig. S1 Aluminum-nickel binary phase diagram (Ni weight percent ranging from 0 to about 70 wt.%) adopted from Ref.1
II. Sample preparation
Preparation of metal alloys
Before melting, aluminum and nickel foils (1.0 mm thick, 99.999% trace metals basis, Aldrich,
Germany) of required weight were folded together and pressed into a rectangle-shaped pellet.
Upon cooling of the melt, newly prepared alloy was pressed into a plate and folded back to the
rectangular shape followed by re-melting. The entire procedure was repeated four times to
ensure that aluminum and nickel have been completely mixed. Melting and cooling steps in
alloy preparation were performed in argon atmosphere to prevent oxidation. The final alloy
Electronic Supplementary Material (ESI) for Green Chemistry.This journal is The Royal Society of Chemistry 2015
plate was processed in the milling machine (Rotormhle Fritsch Pulverisette 14) and meshed
towards obtaining an alloy powder with an average particle size of ~140 m. The pure
intermetallic phases, Al3Ni2 and Al3Ni (~150 m), have been supplied by Goodfellow GmbH
(Germany). The powder X-ray diffractions (PXRD) of the pure phases are shown in Fig. S2.
Fig.S2 PXRD patterns of the pure phases.
High Power Ultrasound (HPUS) treatment of metal alloys
The sonication cell is shown in Fig. S3.
AlNi alloy (powder suspension)
Fig. S3 Photo of the cell for HPUS treatment of the AlNi powdered alloys.
AlNi powder (4g) was dispersed in 40 mL ethanol and sonicated for 60 min with a Hielscher
UIP1000hd, (Hielscher Ultrasonics GmbH, Germany) operated at 20 kHz with a maximum
output power of 1000 W. The apparatus is equipped with an ultrasonic horn BS2d22 (head
area of 3.8 cm2) and a booster B2-1.8. The maximum intensity was calculated to be 140 W
cm2 at mechanical amplitude of 140 m. To avoid overheating during sonication the
experiment was carried out in a homemade thermostatic cell connected to a thermostat
(Huber GmbH, Germany). The temperature was monitored during the treatment and kept at
298 K. After the HPUS treatment, the metal particles were separated from the supernatant by
centrifugation at a speed of 10 000 rpm for 1h and washed with absolute ethanol followed by
drying in vacuum at room temperature.2
I. Sample characterization
For electrochemical measurements a three-electrode cell consisting of Ag/AgCl/
(saturated KCl) reference electrode (potential was converted to standard hydrogen electrode
(SHE)), the Pt foil (6 cm2) counter electrode, and paraffin impregnated graphite electrode
(PIGE) as a working electrode was employed. HIUS modified AlNi alloy particles were
immobilized on PIGE with use of Nafion as a binder solution. Linear Sweep Voltammetry
(LSV) measurements were performed on a 510 V10 Potentiostat/Galvanostat
(MaterialMates, Italy) in the potential region -0.2V to-0.9V with a scan rate of 50mV/s and
use of 1M H2SO4 as a supporting electrolyte.
To determine lifetime performance of the ultrasonically treated catalyst for HER,
galvanostatic responses were recorded at 60 mA/cm2 for 9 consecutive hours.
27Al Magic Angle Spinning Nuclear Magnetic Resonance (MAS NMR)
The solid state 27Al NMR spectra were recorded on a Bruker AvanceII 300 tuned to a
resonance frequency of 78.2 (7.04 T). All magic angle spinning (MAS) NMR experiments
were carried out with a commercial 2.5 mm triple resonance MAS probe operating with
spinning speed of 20 kHz. The chemical shifts are reported with respect to a solution of
AlCl3 adjusted to a pH of 1 with HCl (iso = 0 ppm). All spectra were acquired using a single
pulse excitation with a pulse length of 1.5 s and a recycle delay of 0.2 s. To assure a
selective excitation of the central transition, the corresponding nutation frequency was
adjusted to 16.7 kHz based on the AlCl3 reference solution.
27Al MAS NMR spectroscopy was used to identify the individual intermetallic phases near
the surfaces of the AlNi nanoparticles. The sensitivity towards the surfaces arises from the
skin effect.3 It describes the ability of the radio-frequency (rf) field to penetrate into
conducting and magnetic material, respectively. The skin depth, d, is proportional to
0-1/2, r-1/2 and 1/2 with 0 being the Lamor frequency, r being the relative permeability and
being the electric resistance. While 0 is constant for all experiments, and r might vary
for the individual AlxNiy phases studied here. In particular, r is 2-3orders of magnitude
higher for ferromagnetic materials, as compared to Pauli paramagnets, such as metallic
aluminum. However, due to the gradual changes observed for the pristine and sonicated
materials no strong influence on the skin depth is expected rendering 27Al NMR into a semi-
quantitative technique in this case. Thus a tentative interpretation of the spectral intensities in
terms of phase composition should be possible.
While metallic Al depicts a sharp resonance at 1640 ppm, Al3Ni is characterized by two
broad peaks at 940 ppm and 640 ppm with an intensity ratio of 1:2. Al3Ni2 exhibits single
resonance at 340 ppm. All three resonances depict a line shape typical for a second order
quadrupolar broadening (Fig. 4e, f). The experimental 27Al isotropic chemical shift (iso),
nuclear quadrupole coupling constants (Cq), anisotropy (q), and the individual contributions
from each AlNi phases in atomic percentage are tabulated in the Table S1.
Table. S1: 27Al NMR chemical shift, nuclear quadrupole coupling constants (Cq), anisotropy (q) and the individual contributions (at%) from each phase of AlNi alloy.
AlNi(50/50) Parameters Metallic Al Al3Ni-site 1 Al3Ni-site 2 Al3Ni2 Al(OH)3
iso / ppm 1638.0 940.0 641.0 340.0 0.0
Cq / kHz -- 9151.73 9026.70 8822.00 --
q -- 0.55 0.59 0.67 --Initial
at% 26.23% 13.9% 32.94% 25.65% 1.23%
Cq / kHz -- 9787.72 8948.54 8956.11 --
q -- 0.57 0.60 0.69 --Sonicated
at% 27.01% 15.57% 29.01% 27.05% 1.37%
Transmission electron microscopy (TEM) and selected area electron diffractions (SAED)
were performed with a LEO 922 EFTEM instrument operating at 200 kV.
Scanning electron microscopy (SEM) and energy dispersive X-ray spectroscopy (EDS)
measurements were carried outwith a Gemini Leo 1550 instrument at an operating voltage of
3keV. The results of surface chemical analysis for the pristine AlNi alloy (50 wt.% of Ni) are
shown in Table S2.
Table S2. EDS analysis of the surface of the initial AlNi (50 wt.% Ni) particles.
Al Ni Al:Ni
Analyzed area 1 21.40 28.10 1:1.3
Analyzed area 2 32.70 22.87 3:2
Analyzed area 3 28.75 44.65 2:3
Powder X-ray diffraction (PXRD) measurements with intermetallic samples were carried out
by the aid of a Stoe STADI P X-ray transmission diffractometer, equipped with a Cu sealed
tube and built-in Ni filter (Cu K radiation, = 1.54056 ). The phase composition was
estimated using Rietvild refinement.
The PXRD profiles, as functions of double Btagg angle, 2 are shown in Fig. S4. For
extracting important crystallographic information, i.e. crystallite size, D, and average
microstrain fluctuations, ,we used the standard Williamson Hall (W-H) approach.4-6
In the W-H method, the measured widths, , of diffraction peaks with Miller indices, hkl,
(after applying instrumental correction), are presented in the following form:
= ( ) + (4)where shape factor k = 0.94. It is worth to mention that only non-overlapping diffraction
peaks were used by us for this analysis. The classical W-H equation assumes that the
microstrain fluctuations, , are independent of crystallographic direction.
Fig. S4 Powder X-ray diffraction patterns of the initial (solid line) and ultrasonically modified (dashed line) AlNi (Ni50 wt.%) with evidence for peak narrowing (insets).
The temperature effect on crystal size of the intermetallics in AlNi particles
Fig. S5 shows the dependence of the crystal sizes of Al3Ni2 and Al3Ni phases in the samples
that were heated in oven for 1 h at different temperatures. We see that up to 700C the size of
the crystals strongly depends on the applied temperature, while above this temperature some
kind of saturation is reached. Placing the crystal size of the sonicated samples on this plot,
we can estimate the effective temperature that is achieved within metal particles upon HPUS.
Thus estimated average effective temperature in the sonicated particles was found to be
about ~550C (823 K).
As is seen in the right-hand panel in Figure S5, above 800C (1073 K) the Al3Ni phase is
disappeared, i.e. is transformed into the Al3Ni2 phase. Thus, ultrasonication is able